#------------------------------------------------------------------------------
#$Date: 2025-07-01 13:44:25 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1119 $
#$URL: svn://crystallography.net/testcod/cif/2/00/00/2000017.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2000017
loop_
_publ_author_name
'Strange, Nicholas A.'
'Bell, Robert T.'
'Park, James Eujin'
'Stone, Kevin H.'
'Coker, Eric N.'
'Ginley, David S.'
_publ_section_title
;
 Formation of Ba3Nb0.75Mn2.25O9-6H during thermochemical reduction of
 Ba4NbMn3O12-12R
;
_journal_issue                   5
_journal_name_full
'Acta Crystallographica Section E Crystallographic Communications'
_journal_page_first              469
_journal_page_last               473
_journal_paper_doi               10.1107/S2056989023003213
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'Ba Mn0.5 Nb0.5 O3'
_chemical_formula_weight         259.2474
_space_group_crystal_system      cubic
_space_group_IT_number           221
_space_group_name_Hall           '-P 4 2 3'
_space_group_name_H-M_alt        'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.10182(5)
_cell_length_b                   4.10182(5)
_cell_length_c                   4.10182(5)
_cell_measurement_reflns_used    353
_cell_measurement_temperature    300
_cell_measurement_theta_max      41.75
_cell_measurement_theta_min      2.5
_cell_volume                     69.0128(15)
_diffrn_ambient_temperature      300
_diffrn_measured_fraction_theta_full 30
_diffrn_measurement_device_type  SSRL_beamline_2-1
_diffrn_radiation_wavelength     0.729276500
_exptl_absorpt_coefficient_mu    19.447
_exptl_crystal_density_diffrn    6.2378(2)
_pd_block_diffractogram_id       Bell_BNM_1350_0ppmO2_scan1
_pd_block_id                     barium_niobiumV_manganeseIII_oxide
_pd_phase_name                   BaNb0.5Mn0.5O3
_cod_data_source_file            wm5677sup2.txt
_cod_data_source_block           barium_niobiumV_manganeseIII_oxide
_cod_original_cell_volume        69.013(2)
_cod_original_sg_symbol_H-M      Pm-3m
_cod_original_formula_sum        BaNb0.5Mn0.5O3
_cod_database_code               2000017
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z '
2 '-x, -y, z '
3 '-x, -z, -y '
4 '-x, -z, y '
5 '-x, z, -y '
6 '-x, z, y '
7 '-x, y, -z '
8 '-x, y, z '
9 '-y, -x, -z '
10 '-y, -x, z '
11 '-y, -z, -x '
12 '-y, -z, x '
13 '-y, z, -x '
14 '-y, z, x '
15 '-y, x, -z '
16 '-y, x, z '
17 '-z, -x, -y '
18 '-z, -x, y '
19 '-z, -y, -x '
20 '-z, -y, x '
21 '-z, y, -x '
22 '-z, y, x '
23 '-z, x, -y '
24 '-z, x, y '
25 'z, -x, -y '
26 'z, -x, y '
27 'z, -y, -x '
28 'z, -y, x '
29 'z, y, -x '
30 'z, y, x '
31 'z, x, -y '
32 'z, x, y '
33 'y, -x, -z '
34 'y, -x, z '
35 'y, -z, -x '
36 'y, -z, x '
37 'y, z, -x '
38 'y, z, x '
39 'y, x, -z '
40 'y, x, z '
41 'x, -y, -z '
42 'x, -y, z '
43 'x, -z, -y '
44 'x, -z, y '
45 'x, z, -y '
46 'x, z, y '
47 'x, y, -z '
48 '-x, -y, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ba1 Ba+2 1 0 0 0 1 0.1
Mn1 Mn+3 1 0.5 0.5 0.5 0.5 0.1
Nb1 Nb+5 1 0.5 0.5 0.5 0.5 0.1
O1 O-2 3 0.5 0.5 0 1 0.1
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
O1 Ba1 O1 60.000 3_655 1_555 17_565
O1 Ba1 O1 60.000 1_545 1_555 3_655
O1 Ba1 O1 120.000 1_545 1_555 17_565
O1 Ba1 O1 180.000 1_455 1_555 1_545
O1 Ba1 O1 120.000 1_455 1_555 3_655
O1 Ba1 O1 60.000 1_455 1_555 17_565
O1 Ba1 O1 120.000 17_556 1_555 1_455
O1 Ba1 O1 60.000 17_556 1_555 1_545
O1 Ba1 O1 120.000 17_556 1_555 3_655
O1 Ba1 O1 180.000 17_556 1_555 17_565
O1 Ba1 O1 60.000 3_556 1_555 17_556
O1 Ba1 O1 60.000 3_556 1_555 1_455
O1 Ba1 O1 120.000 3_556 1_555 1_545
O1 Ba1 O1 180.000 3_556 1_555 3_655
O1 Ba1 O1 120.000 3_556 1_555 17_565
O1 Ba1 O1 60.000 17_566 1_555 3_556
O1 Ba1 O1 90.000 17_566 1_555 17_556
O1 Ba1 O1 60.000 17_566 1_555 1_455
O1 Ba1 O1 120.000 17_566 1_555 1_545
O1 Ba1 O1 120.000 17_566 1_555 3_655
O1 Ba1 O1 90.000 17_566 1_555 17_565
O1 Ba1 O1 60.000 3_656 1_555 17_566
O1 Ba1 O1 90.000 3_656 1_555 3_556
O1 Ba1 O1 60.000 3_656 1_555 17_556
O1 Ba1 O1 120.000 3_656 1_555 1_455
O1 Ba1 O1 60.000 3_656 1_555 1_545
O1 Ba1 O1 90.000 3_656 1_555 3_655
O1 Ba1 O1 120.000 3_656 1_555 17_565
O1 Ba1 O1 60.000 1_555 1_555 3_656
O1 Ba1 O1 60.000 1_555 1_555 17_566
O1 Ba1 O1 120.000 1_555 1_555 3_556
O1 Ba1 O1 120.000 1_555 1_555 17_556
O1 Ba1 O1 90.000 1_555 1_555 1_455
O1 Ba1 O1 90.000 1_555 1_555 1_545
O1 Ba1 O1 60.000 1_555 1_555 3_655
O1 Ba1 O1 60.000 1_555 1_555 17_565
O1 Ba1 O1 120.000 17_555 1_555 1_555
O1 Ba1 O1 120.000 17_555 1_555 3_656
O1 Ba1 O1 180.000 17_555 1_555 17_566
O1 Ba1 O1 120.000 17_555 1_555 3_556
O1 Ba1 O1 90.000 17_555 1_555 17_556
O1 Ba1 O1 120.000 17_555 1_555 1_455
O1 Ba1 O1 60.000 17_555 1_555 1_545
O1 Ba1 O1 60.000 17_555 1_555 3_655
O1 Ba1 O1 90.000 17_555 1_555 17_565
O1 Ba1 O1 60.000 3_555 1_555 17_555
O1 Ba1 O1 120.000 3_555 1_555 1_555
O1 Ba1 O1 179.99999879(14) 3_555 1_555 3_656
O1 Ba1 O1 120.000 3_555 1_555 17_566
O1 Ba1 O1 90.000 3_555 1_555 3_556
O1 Ba1 O1 120.000 3_555 1_555 17_556
O1 Ba1 O1 60.000 3_555 1_555 1_455
O1 Ba1 O1 120.000 3_555 1_555 1_545
O1 Ba1 O1 90.000 3_555 1_555 3_655
O1 Ba1 O1 60.000 3_555 1_555 17_565
O1 Ba1 O1 60.000 1_445 1_555 3_555
O1 Ba1 O1 60.000 1_445 1_555 17_555
O1 Ba1 O1 180.000 1_445 1_555 1_555
O1 Ba1 O1 120.000 1_445 1_555 3_656
O1 Ba1 O1 120.000 1_445 1_555 17_566
O1 Ba1 O1 60.000 1_445 1_555 3_556
O1 Ba1 O1 60.000 1_445 1_555 17_556
O1 Ba1 O1 90.000 1_445 1_555 1_455
O1 Ba1 O1 90.000 1_445 1_555 1_545
O1 Ba1 O1 120.000 1_445 1_555 3_655
O1 Ba1 O1 120.000 1_445 1_555 17_565
O1 Mn1 Nb1 . 3_666 1_555 1_555
O1 Mn1 O1 90.000 17_666 1_555 3_666
O1 Mn1 Nb1 . 17_666 1_555 1_555
O1 Mn1 O1 90.000 3_656 1_555 17_666
O1 Mn1 O1 180.00000000(14) 3_656 1_555 3_666
O1 Mn1 Nb1 . 3_656 1_555 1_555
O1 Mn1 O1 90.000 1_555 1_555 3_656
O1 Mn1 O1 90.000 1_555 1_555 17_666
O1 Mn1 O1 90.000 1_555 1_555 3_666
O1 Mn1 Nb1 . 1_555 1_555 1_555
O1 Mn1 O1 180.000 1_556 1_555 1_555
O1 Mn1 O1 90.000 1_556 1_555 3_656
O1 Mn1 O1 90.000 1_556 1_555 17_666
O1 Mn1 O1 90.000 1_556 1_555 3_666
O1 Mn1 Nb1 . 1_556 1_555 1_555
O1 Mn1 O1 90.000 17_566 1_555 1_556
O1 Mn1 O1 90.000 17_566 1_555 1_555
O1 Mn1 O1 90.000 17_566 1_555 3_656
O1 Mn1 O1 180.000 17_566 1_555 17_666
O1 Mn1 O1 90.000 17_566 1_555 3_666
O1 Mn1 Nb1 . 17_566 1_555 1_555
O1 Nb1 Mn1 . 3_666 1_555 1_555
O1 Nb1 O1 90.000 17_666 1_555 3_666
O1 Nb1 Mn1 . 17_666 1_555 1_555
O1 Nb1 O1 90.000 3_656 1_555 17_666
O1 Nb1 O1 180.00000000(14) 3_656 1_555 3_666
O1 Nb1 Mn1 . 3_656 1_555 1_555
O1 Nb1 O1 90.000 1_555 1_555 3_656
O1 Nb1 O1 90.000 1_555 1_555 17_666
O1 Nb1 O1 90.000 1_555 1_555 3_666
O1 Nb1 Mn1 . 1_555 1_555 1_555
O1 Nb1 O1 180.000 1_556 1_555 1_555
O1 Nb1 O1 90.000 1_556 1_555 3_656
O1 Nb1 O1 90.000 1_556 1_555 17_666
O1 Nb1 O1 90.000 1_556 1_555 3_666
O1 Nb1 Mn1 . 1_556 1_555 1_555
O1 Nb1 O1 90.000 17_566 1_555 1_556
O1 Nb1 O1 90.000 17_566 1_555 1_555
O1 Nb1 O1 90.000 17_566 1_555 3_656
O1 Nb1 O1 180.000 17_566 1_555 17_666
O1 Nb1 O1 90.000 17_566 1_555 3_666
O1 Nb1 Mn1 . 17_566 1_555 1_555
Mn1 O1 Mn1 180.000 1_554 1_555 1_555
Nb1 O1 Mn1 180.000 1_555 1_555 1_554
Nb1 O1 Mn1 0.000 1_555 1_555 1_555
Nb1 O1 Nb1 180.000 1_554 1_555 1_555
Nb1 O1 Mn1 0.000 1_554 1_555 1_554
Nb1 O1 Mn1 180.000 1_554 1_555 1_555
Ba1 O1 Nb1 90.000 1_655 1_555 1_554
Ba1 O1 Nb1 90.000 1_655 1_555 1_555
Ba1 O1 Mn1 90.000 1_655 1_555 1_554
Ba1 O1 Mn1 90.000 1_655 1_555 1_555
Ba1 O1 Ba1 180.000 1_565 1_555 1_655
Ba1 O1 Nb1 90.000 1_565 1_555 1_554
Ba1 O1 Nb1 90.000 1_565 1_555 1_555
Ba1 O1 Mn1 90.000 1_565 1_555 1_554
Ba1 O1 Mn1 90.000 1_565 1_555 1_555
O1 O1 Ba1 60.000 3_665 1_555 1_565
O1 O1 Ba1 120.000 3_665 1_555 1_655
O1 O1 Nb1 45.000 3_665 1_555 1_554
O1 O1 Nb1 135.000 3_665 1_555 1_555
O1 O1 Mn1 45.000 3_665 1_555 1_554
O1 O1 Mn1 135.000 3_665 1_555 1_555
O1 O1 O1 60.000 17_665 1_555 3_665
O1 O1 Ba1 120.000 17_665 1_555 1_565
O1 O1 Ba1 60.000 17_665 1_555 1_655
O1 O1 Nb1 45.000 17_665 1_555 1_554
O1 O1 Nb1 135.000 17_665 1_555 1_555
O1 O1 Mn1 45.000 17_665 1_555 1_554
O1 O1 Mn1 135.000 17_665 1_555 1_555
O1 O1 O1 120.000 3_656 1_555 17_665
O1 O1 O1 180.000 3_656 1_555 3_665
O1 O1 Ba1 120.000 3_656 1_555 1_565
O1 O1 Ba1 60.000 3_656 1_555 1_655
O1 O1 Nb1 135.000 3_656 1_555 1_554
O1 O1 Nb1 45.000 3_656 1_555 1_555
O1 O1 Mn1 135.000 3_656 1_555 1_554
O1 O1 Mn1 45.000 3_656 1_555 1_555
O1 O1 O1 60.000 17_566 1_555 3_656
O1 O1 O1 180.00000000(14) 17_566 1_555 17_665
O1 O1 O1 120.000 17_566 1_555 3_665
O1 O1 Ba1 60.000 17_566 1_555 1_565
O1 O1 Ba1 120.000 17_566 1_555 1_655
O1 O1 Nb1 135.000 17_566 1_555 1_554
O1 O1 Nb1 45.000 17_566 1_555 1_555
O1 O1 Mn1 135.000 17_566 1_555 1_554
O1 O1 Mn1 45.000 17_566 1_555 1_555
Ba1 O1 O1 120.000 1_665 1_555 17_566
Ba1 O1 O1 120.000 1_665 1_555 3_656
Ba1 O1 O1 60.000 1_665 1_555 17_665
Ba1 O1 O1 60.000 1_665 1_555 3_665
Ba1 O1 Ba1 90.000 1_665 1_555 1_565
Ba1 O1 Ba1 90.000 1_665 1_555 1_655
Ba1 O1 Nb1 90.000 1_665 1_555 1_554
Ba1 O1 Nb1 90.000 1_665 1_555 1_555
Ba1 O1 Mn1 90.000 1_665 1_555 1_554
Ba1 O1 Mn1 90.000 1_665 1_555 1_555
O1 O1 Ba1 60.000 3_666 1_555 1_665
O1 O1 O1 60.000 3_666 1_555 17_566
O1 O1 O1 90.000 3_666 1_555 3_656
O1 O1 O1 120.000 3_666 1_555 17_665
O1 O1 O1 90.000 3_666 1_555 3_665
O1 O1 Ba1 60.000 3_666 1_555 1_565
O1 O1 Ba1 120.000 3_666 1_555 1_655
O1 O1 Nb1 135.000 3_666 1_555 1_554
O1 O1 Nb1 45.000 3_666 1_555 1_555
O1 O1 Mn1 135.000 3_666 1_555 1_554
O1 O1 Mn1 45.000 3_666 1_555 1_555
O1 O1 O1 60.000 17_666 1_555 3_666
O1 O1 Ba1 60.000 17_666 1_555 1_665
O1 O1 O1 90.000 17_666 1_555 17_566
O1 O1 O1 60.000 17_666 1_555 3_656
O1 O1 O1 90.000 17_666 1_555 17_665
O1 O1 O1 120.000 17_666 1_555 3_665
O1 O1 Ba1 120.000 17_666 1_555 1_565
O1 O1 Ba1 60.000 17_666 1_555 1_655
O1 O1 Nb1 135.000 17_666 1_555 1_554
O1 O1 Nb1 45.000 17_666 1_555 1_555
O1 O1 Mn1 135.000 17_666 1_555 1_554
O1 O1 Mn1 45.000 17_666 1_555 1_555
O1 O1 O1 120.000 3_655 1_555 17_666
O1 O1 O1 180.00000000(14) 3_655 1_555 3_666
O1 O1 Ba1 120.000 3_655 1_555 1_665
O1 O1 O1 120.000 3_655 1_555 17_566
O1 O1 O1 90.000 3_655 1_555 3_656
O1 O1 O1 60.000 3_655 1_555 17_665
O1 O1 O1 90.000 3_655 1_555 3_665
O1 O1 Ba1 120.000 3_655 1_555 1_565
O1 O1 Ba1 60.000 3_655 1_555 1_655
O1 O1 Nb1 45.000 3_655 1_555 1_554
O1 O1 Nb1 135.000 3_655 1_555 1_555
O1 O1 Mn1 45.000 3_655 1_555 1_554
O1 O1 Mn1 135.000 3_655 1_555 1_555
O1 O1 O1 60.000 17_565 1_555 3_655
O1 O1 O1 179.99999879(14) 17_565 1_555 17_666
O1 O1 O1 120.000 17_565 1_555 3_666
O1 O1 Ba1 120.000 17_565 1_555 1_665
O1 O1 O1 90.000 17_565 1_555 17_566
O1 O1 O1 120.000 17_565 1_555 3_656
O1 O1 O1 90.000 17_565 1_555 17_665
O1 O1 O1 60.000 17_565 1_555 3_665
O1 O1 Ba1 60.000 17_565 1_555 1_565
O1 O1 Ba1 120.000 17_565 1_555 1_655
O1 O1 Nb1 45.000 17_565 1_555 1_554
O1 O1 Nb1 135.000 17_565 1_555 1_555
O1 O1 Mn1 45.000 17_565 1_555 1_554
O1 O1 Mn1 135.000 17_565 1_555 1_555
Ba1 O1 O1 60.000 1_555 1_555 17_565
Ba1 O1 O1 60.000 1_555 1_555 3_655
Ba1 O1 O1 120.000 1_555 1_555 17_666
Ba1 O1 O1 120.000 1_555 1_555 3_666
Ba1 O1 Ba1 180.00000000(14) 1_555 1_555 1_665
Ba1 O1 O1 60.000 1_555 1_555 17_566
Ba1 O1 O1 60.000 1_555 1_555 3_656
Ba1 O1 O1 120.000 1_555 1_555 17_665
Ba1 O1 O1 120.000 1_555 1_555 3_665
Ba1 O1 Ba1 90.000 1_555 1_555 1_565
Ba1 O1 Ba1 90.000 1_555 1_555 1_655
Ba1 O1 Nb1 90.000 1_555 1_555 1_554
Ba1 O1 Nb1 90.000 1_555 1_555 1_555
Ba1 O1 Mn1 90.000 1_555 1_555 1_554
Ba1 O1 Mn1 90.000 1_555 1_555 1_555
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Ba1 O1 2.90042(3) 1_555 17_565
Ba1 O1 2.90042(3) 1_555 3_655
Ba1 O1 2.90042(3) 1_555 1_545
Ba1 O1 2.90042(3) 1_555 1_455
Ba1 O1 2.90042(3) 1_555 17_556
Ba1 O1 2.90042(3) 1_555 3_556
Ba1 O1 2.90042(3) 1_555 17_566
Ba1 O1 2.90042(3) 1_555 3_656
Ba1 O1 2.90042(3) 1_555 1_555
Ba1 O1 2.90042(3) 1_555 17_555
Ba1 O1 2.90042(3) 1_555 3_555
Ba1 O1 2.90042(3) 1_555 1_445
Mn1 Nb1 0.00000 1_555 1_555
Mn1 O1 2.05091(2) 1_555 3_666
Mn1 O1 2.05091(2) 1_555 17_666
Mn1 O1 2.05091(2) 1_555 3_656
Mn1 O1 2.05091(2) 1_555 1_555
Mn1 O1 2.05091(2) 1_555 1_556
Mn1 O1 2.05091(2) 1_555 17_566
Nb1 Mn1 0.00000 1_555 1_555
Nb1 O1 2.05091(2) 1_555 3_666
Nb1 O1 2.05091(2) 1_555 17_666
Nb1 O1 2.05091(2) 1_555 3_656
Nb1 O1 2.05091(2) 1_555 1_555
Nb1 O1 2.05091(2) 1_555 1_556
Nb1 O1 2.05091(2) 1_555 17_566
O1 Mn1 2.05091(2) 1_555 1_555
O1 Mn1 2.05091(2) 1_555 1_554
O1 Nb1 2.05091(2) 1_555 1_555
O1 Nb1 2.05091(2) 1_555 1_554
O1 Ba1 2.90042(3) 1_555 1_655
O1 Ba1 2.90042(3) 1_555 1_565
O1 O1 2.90042(3) 1_555 3_665
O1 O1 2.90042(3) 1_555 17_665
O1 O1 2.90042(3) 1_555 3_656
O1 O1 2.90042(3) 1_555 17_566
O1 Ba1 2.90042(3) 1_555 1_665
O1 O1 2.90042(3) 1_555 3_666
O1 O1 2.90042(3) 1_555 17_666
O1 O1 2.90042(3) 1_555 3_655
O1 O1 2.90042(3) 1_555 17_565
O1 Ba1 2.90042(3) 1_555 1_555
